Quantum spin liquid: design of a quantum spin liquid next to a superconducting state based on a dimer-type ET Mott insulator
Takaaki Hiramatsu; Yukihiro Yoshida; Gunzi Saito; Akihiro Otsuka; Hideki Yamochi; Mitsuhiko Maesato; Yasuhiro Shimizu; Hiroshi Ito; Hideo Kishida; Journal of Materials Chemistry C 3 (2015) 1378–1388; doi:10.1039/C4TC01701C

data_7234072
_publ_section_title
;
 Quantum spin liquid: design of a quantum spin liquid next to a
 superconducting state based on a dimer-type ET Mott insulator
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              1378
_journal_page_last               1388
_journal_paper_doi               10.1039/C4TC01701C
_journal_volume                  3
_journal_year                    2015
_chemical_formula_moiety         '2(C10 H8 S8), C2 Ag1 N2, H2 O1'
_chemical_formula_sum            'C22 H18 Ag N2 O S16'
_chemical_formula_weight         947.21
_chemical_name_common
;
bis(bis(Ethylenedithio)tetrathiafulvalene) dicyano-silver monohydrate
;
_chemical_name_systematic
;
bis(3,4;3',4'-bis(Ethylenedithio)-2,2',5,5'-tetrathiafulvalenium)
dicyano-silver(i) monohydrate
;
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 109.6200(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   16.0283(11)
_cell_length_b                   8.5985(6)
_cell_length_c                   12.5042(8)
_cell_measurement_reflns_used    9848
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      28.26
_cell_measurement_theta_min      2.53
_cell_volume                     1623.27(19)
_computing_cell_refinement       'APEX2 (Bruker AXS, 2006)'
_computing_data_collection       'APEX2 '
_computing_data_reduction        'SAINT (Bruker AXS, 2004)'
_computing_publication_material
'Yadokari-XG 2009 (Wakita, Nemoto et al., 2009)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEXII CCD area detector'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0104
_diffrn_reflns_av_sigmaI/netI    0.0164
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            17764
_diffrn_reflns_theta_full        27.00
_diffrn_reflns_theta_max         27.00
_diffrn_reflns_theta_min         1.35
_exptl_absorpt_coefficient_mu    1.677
_exptl_absorpt_correction_T_max  0.8371
_exptl_absorpt_correction_T_min  0.6911
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
APEX2 Software
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.938
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'rectangular needle'
_exptl_crystal_F_000             950
_exptl_crystal_preparation       'Magnetic properties, electronic property'
_exptl_crystal_recrystallization_method electrocrystallization
_exptl_crystal_size_max          0.34
_exptl_crystal_size_mid          0.33
_exptl_crystal_size_min          0.11
_refine_diff_density_max         0.585
_refine_diff_density_min         -0.832
_refine_diff_density_rms         0.051
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.018(13)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.105
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     379
_refine_ls_number_reflns         7009
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.104
_refine_ls_R_factor_all          0.0177
_refine_ls_R_factor_gt           0.0173
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0197P)^2^+0.6113P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0445
_refine_ls_wR_factor_ref         0.0447
_reflns_number_gt                6897
_reflns_number_total             7009
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            1000028.cif
_cod_data_source_block           PCOD1000028
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Monoclinic' was changed to
'monoclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        1623.26(19)
_cod_original_sg_symbol_H-M      'P2(1)   '
_cod_database_code               7234072